A ferroelectric proton conductor with colossal polarization induced by in-plane symmetry breaking in a two-dimensional coordination polymer.
Song, Yanqing; Tsuji, Yuta; Sugimoto, Kunihisa; Kikuchi, Takashi; Shi, Yuxin; Murakami, Yusuke; Hiramatsu, Kotaro; Le Ouay, Benjamin; Ohba, Masaaki; Ohtani, Ryo; Chemical science 16 (2025) 13413–13421; doi:10.1039/d4sc08700c

data_1574943
_publ_section_title
;
 A ferroelectric proton conductor with colossal polarization induced by
 in-plane symmetry breaking in a two-dimensional coordination polymer.
;
_journal_issue                   29
_journal_name_full               'Chemical science'
_journal_page_first              13413
_journal_page_last               13421
_journal_paper_doi               10.1039/d4sc08700c
_journal_volume                  16
_journal_year                    2025
_chemical_formula_moiety         'C38 H26 Mn2 N10 O4 Re'
_chemical_formula_sum            'C38 H26 Mn2 N10 O4 Re'
_chemical_formula_weight         982.77
_space_group_crystal_system      tetragonal
_space_group_IT_number           85
_space_group_name_Hall           '-P 4a'
_space_group_name_H-M_alt        'P 4/n :2'
_atom_sites_solution_hydrogens   geom
_audit_creation_date             2024-11-19
_audit_creation_method
;
Olex2 1.5
(compiled 2024.02.16 svn.r378c4104 for OlexSys, GUI svn.r6928)
;
_audit_update_record
;
2024-12-16 deposited with the CCDC.	2025-06-02 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   14.3719(3)
_cell_length_b                   14.3719(3)
_cell_length_c                   18.0827(6)
_cell_measurement_reflns_used    11376
_cell_measurement_temperature    150
_cell_measurement_theta_max      30.4500
_cell_measurement_theta_min      2.6040
_cell_volume                     3735.01(17)
_computing_cell_refinement       'CrysAlisPro 1.171.39.46e (Rigaku OD, 2018)'
_computing_data_collection       'CrysAlisPro 1.171.39.46e (Rigaku OD, 2018)'
_computing_data_reduction        'CrysAlisPro 1.171.39.46e (Rigaku OD, 2018)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_diffrn_ambient_temperature      150
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.873
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  t~exp~   \w     \q     \k     \f   Frames
  1  \w    -61.00 -35.00   0.50    2.00    --  -10.20  45.00  30.00   52
  2  \w     20.00  60.00   0.50    2.00    --  -10.20  45.00  30.00   80
  3  \w    -99.00   7.00   0.50    2.00    --  -10.20  45.00  60.00  212
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'XtaLAB AFC10 (RCD3): fixed-chi single'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0248
_diffrn_reflns_av_unetI/netI     0.0261
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.873
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_number            20242
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.873
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         31.037
_diffrn_reflns_theta_min         2.299
_exptl_absorpt_coefficient_mu    3.954
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.70414
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.39.46e (Rigaku Oxford Diffraction, 2018)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            brown
_exptl_crystal_density_diffrn    1.748
_exptl_crystal_description       block
_exptl_crystal_F_000             1924
_exptl_crystal_size_max          0.3
_exptl_crystal_size_mid          0.3
_exptl_crystal_size_min          0.2
_refine_diff_density_max         5.091
_refine_diff_density_min         -3.617
_refine_diff_density_rms         0.214
_refine_ls_extinction_coef       0.0043(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2018/3 (Sheldrick 2018)'
_refine_ls_goodness_of_fit_ref   1.131
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     349
_refine_ls_number_reflns         5233
_refine_ls_number_restraints     353
_refine_ls_restrained_S_all      1.129
_refine_ls_R_factor_all          0.0639
_refine_ls_R_factor_gt           0.0590
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0527P)^2^+38.3924P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1482
_refine_ls_wR_factor_ref         0.1506
_reflns_Friedel_coverage         0.000
_reflns_number_gt                4760
_reflns_number_total             5233
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d4sc08700c2.cif
_cod_data_source_block           mnremecn_150_c_2
_cod_depositor_comments
'Adding full bibliography for 1574937--1574947.cif.'
_cod_original_cell_volume        3735.0(2)
_cod_original_sg_symbol_H-M      'P 4/n'
_cod_database_code               1574943
_shelx_shelxl_version_number     2018/3
_olex2_refinement_description
;
1. Twinned data refinement
 Scales: 0.499(3)
 0.501(3)
2. Fixed Uiso
 At 1.2 times of:
  All C(H) groups, All C(H,H) groups, All C(H,H,H,H) groups
3. Restrained distances
 N8-C21
 1.14 with sigma of 0.02
 C20-N7
 2.593 with sigma of 0.02
 C22-C21
 1.456 with sigma of 0.02
 C19-C20
 1.456 with sigma of 0.01
 N7-C19
 1.14 with sigma of 0.02
 C19-N7
 1.137 with sigma of 0.01
 N8-C22
 2.59 with sigma of 0.04
 N7-C20
 2.59 with sigma of 0.04
 Re2-C18 \\sim Re2-C18A
 with sigma of 0.02
 C18-N4 \\sim C18A-N4A
 with sigma of 0.02
 Mn1-C18 \\sim Mn1-C18A
 with sigma of 0.04
 Re1-C17 \\sim Re1-C17A
 with sigma of 0.02
 Mn1-N3 \\sim Mn1-N3A
 with sigma of 0.02
 C17-N3 \\sim C17A-N3A
 with sigma of 0.02
 N2-C9 \\sim N2A-C9A
 with sigma of 0.02
 Mn1-N4 \\sim Mn1-N4A
 with sigma of 0.02
 C9-C8 \\sim C9A-C8
 with sigma of 0.02
 Mn1-C9 \\sim Mn1-C9A
 with sigma of 0.04
 C9-C10 \\sim C9A-C10A
 with sigma of 0.04
 Re1-N3 \\sim Re1-N3A
 with sigma of 0.04
 Re2-N4 \\sim Re2-N4A
 with sigma of 0.04
 Mn1-C17 \\sim Mn1-C17A
 with sigma of 0.04
 Mn1-N2 \\sim Mn1-N2A
 with sigma of 0.02
 C14-C13 \\sim C14-C13A
 with sigma of 0.02
 C16-C11 \\sim C16-C11A
 with sigma of 0.02
 C11-C12 \\sim C11A-C12A
 with sigma of 0.02
 C11-C10 \\sim C11A-C10A
 with sigma of 0.02
 N2-C10 \\sim N2A-C10A
 with sigma of 0.02
 C13-C12 \\sim C13A-C12A
 with sigma of 0.02
 Mn1-C10 \\sim Mn1-C10A
 with sigma of 0.04
 C14-C12 \\sim C14-C12A
 with sigma of 0.04
 C16-C12 \\sim C16-C12A
 with sigma of 0.04
 C16-C10 \\sim C16-C10A
 with sigma of 0.04
 C11-N2 \\sim C11A-N2A
 with sigma of 0.04
 C11-C13 \\sim C11A-C13A
 with sigma of 0.04
 N2-C8 \\sim N2A-C8
 with sigma of 0.04
 C12-C10 \\sim C12A-C10A
 with sigma of 0.04
4. Uiso/Uaniso restraints and constraints
N8 \\sim C21 \\sim C22 \\sim Re2: within 2.5A with sigma of 0.02 and sigma for
terminal atoms of 0.04 within 2.5A
N7 \\sim C19 \\sim C20: within 2A with sigma of 0.01 and sigma for terminal
atoms of 0.02 within 2A
Re1 \\sim C17 \\sim N3 \\sim Mn1 \\sim N4A \\sim C18A \\sim Re2: within 2.5A
with sigma of 0.01 and sigma for terminal atoms of 0.02 within 2.5A
Re1 \\sim C17A \\sim N3A \\sim Mn1 \\sim N4 \\sim C18 \\sim Re2: within 2.5A
with sigma of 0.01 and sigma for terminal atoms of 0.02 within 2.5A
Re2 \\sim N6: within 2.5A with sigma of 0.01 and sigma for terminal atoms of
0.02 within 2.5A
C13 \\sim C12 \\sim C11 \\sim C10: within 2A with sigma of 0.01 and sigma for
terminal atoms of 0.02 within 2A
N2 \\sim N1: within 2A with sigma of 0.01 and sigma for terminal atoms of 0.02
within 2A
N1 \\sim C8 \\sim C9 \\sim N2: within 2A with sigma of 0.01 and sigma for
terminal atoms of 0.02 within 2A
C8 \\sim C9A \\sim N2A \\sim C10A \\sim C11A \\sim C12A \\sim C13A: within 2A
with sigma of 0.04 and sigma for terminal atoms of 0.08 within 2A
C8 \\sim C9 \\sim N2 \\sim C10 \\sim C11 \\sim C12 \\sim C13: within 2A with
sigma of 0.04 and sigma for terminal atoms of 0.08 within 2A
Uanis(N8) \\sim Ueq, Uanis(C21) \\sim Ueq, Uanis(C22) \\sim Ueq: with sigma of
0.02 and sigma for terminal atoms of 0.04
Uanis(C18A) \\sim Ueq, Uanis(N4A) \\sim Ueq, Uanis(N4) \\sim Ueq, Uanis(C18)
\\sim Ueq: with sigma of 0.005 and sigma for terminal atoms of 0.01
5. Rigid body (RIGU) restrains
 N8, C21, C22
 with sigma for 1-2 distances of 0.004 and sigma for 1-3 distances of 0.004
 N7, C19, C20
 with sigma for 1-2 distances of 0.004 and sigma for 1-3 distances of 0.004
 Re2, Mn1, C18A, N4A
 with sigma for 1-2 distances of 0.004 and sigma for 1-3 distances of 0.004
 Re2, Mn1, C18, N4
 with sigma for 1-2 distances of 0.004 and sigma for 1-3 distances of 0.004
 N1, C8, C9, N2
 with sigma for 1-2 distances of 0.004 and sigma for 1-3 distances of 0.004
 N2, N1
 with sigma for 1-2 distances of 0.004 and sigma for 1-3 distances of 0.004
 C8, C9A, N2A, C10A, C11A, C12A, C13A
 with sigma for 1-2 distances of 0.004 and sigma for 1-3 distances of 0.004
6. Others
 Sof(C17)=Sof(N3)=Sof(H8BC)=Sof(H8BD)=Sof(C13A)=Sof(H13A)=Sof(C12A)=Sof(H12A)=
 Sof(C11A)=Sof(C10A)=Sof(H10A)=Sof(N2A)=Sof(C9A)=Sof(H9AA)=Sof(H9AB)=Sof(C18A)=
 Sof(N4A)=1-FVAR(1)
 Sof(C18)=Sof(N4)=Sof(C11)=Sof(N2)=Sof(C9)=Sof(H9A)=Sof(H9B)=Sof(H8AA)=
 Sof(H8AB)=Sof(C13)=Sof(H13)=Sof(C12)=Sof(H12)=Sof(C10)=Sof(H10)=Sof(N3A)=
 Sof(C17A)=FVAR(1)
7.a Secondary CH2 refined with riding coordinates:
 C9(H9A,H9B), C8(H8AA,H8AB), C8(H8BC,H8BD), C9A(H9AA,H9AB)
7.b Aromatic/amide H refined with riding coordinates:
 C2(H2), C3(H3), C15(H15), C4(H4), C5(H5), C7(H7), C13(H13), C12(H12),
 C10(H10), C13A(H13A), C12A(H12A), C10A(H10A)
;
_shelx_res_checksum              86251
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;